Copyright to IJIRSET www.ijirset.com 1359
EFFECT OF PULSED CURRENT ON
WELDING CHARACTERISTICS OF EN19
ALLOY STEEL USING GAS TUNGSTEN
, Dr.B.V.R.Ravi Kumar2
Associate Professor, Department of Mechanical Engineering, Malla Reddy Engineering College, Secunderabad, India1
Professor, Department of Mechanical Engineering, VNR.Vignana Jyothi Institute of Engineering & Technology, Hyderabad, India2
Abstract : This paper covers the study of destructive and non-destructive properties of weldments EN19 alloy steel using GTAW with non-pulsed current and pulsed current at different frequencies of 2Hz,4HZ & 6Hz.The radiography, liquid Penetrant test of weldments were evaluated and compared with pulsed and non-pulsed current welding at different frequencies of two different thicknesses of EN19 material (2mm and 3mm ).The aim of this experimental work is to see the effect of pulsed current on the quality of weldments. The experimental results pertaining to different
welding parameters for the above material using pulsed and non-pulsed current GTAW are discussed andcompared.
Keywords: EN19 alloy steel, Gas Tungsten Arc Welding, Constant Current Welding, Pulsed current welding and Heat Affected Zone, Porosity and surface cracks
The demand is increasing for alloy steel weld structures and products where high quality is required such as marine applications. Aluminium alloy, stainless steel and alloy steels can be welded easily by conventional arc welding methods like metal inert gas (MIG) and Tungsten Inert Gas(TIG).Among the two methods ,the gas tungsten arc welding(GTAW)process has proved for many years to be suitable for welding aluminium alloy and alloy steels and stainless steels, since GTAW gives best quality welds. Direct Current Straight Polarity GTAW process is preferred for welding alloy steels. Further development has been pulsed current TIG welding. Pulsed current welding (pcw) was introduced in the late 1960’s as a variant of constant current welding(ccw). pcw process has many advantages over ccw, including enhanced arc stability, increased weld depth/width ratio, narrower HAZ range, reduced hot cracking sensitivity, refined grain size, reduced porosity, low heat input, lower distortion of gas by weld pool and better control of the fusion zone [1-8]. Pulsed current welding technology has been widely used in fabrication of high pressure air bottles, high pressure gas storage tanks, rocket motors, structures in aerospace applications such as aircrafts, rockets and missiles. Switching between predetermined high and low level of welding current can be used to produce pulsed current gas tungsten arc welds.Some progress was there on pulsed current GTAW of aluminium alloy . So far the pulsed current welding is used to study the effect of pulse current , shielding gas composition, weld speed and bead shape , the incidence of welding defects, joint strength , using alloy sheets of 5083 type  angular distortion in SS310 type  , to study the microstructure  and weld bead geometry  .Usually the pulsed waves are in rectangular shape and the parameters used for pulsed GTA welding are is shown in figure 1. The main characteristics of Pulsed Current Welding are determined by peak current Ip base current Ib , peak time tp and base time tb.
II. EXPERIMENTAL PROCEDURE
Copyright to IJIRSET www.ijirset.com 1360
Fig.1 Parameters used for pulsed GTAW: peak current Ip, base current Ib , peak time tp and base time tb. ER80S-B2 filler wire was used during the welding , which reduced the weld cracks and produced the good strength and ductility than other filler metals . These filler metals melt at a temperature lower than that of the base metal. For this reason , it yields during cooling , since it remains more plastic than the base metal and relieves the contraction stresses that might cause cracking. The chemical composition and mechanical properties of work material and filler wire as shown in Tables 1-3.
The alloy steel work pieces were roughly polished with 400 grit abrasive paper and pneumatic rotary brush to remove surface impurities and then clean with Acetone.
A Lincoln Electrical square wave TIG355 GTAW machine with AC & DC was used for welding of EN19specimens .The choice of tungsten electrode depends upon the type of welding current selected for the application. Zirconated tungsten (EWZr) electrodes are best suited for AC wherein they keep hemispherical shape and thoriated tungsten electrodes (EWTh-2) should be ground to taper are suitable for DCSP welding are used for this purpose . This welding process was conducted with 2.5 mm diameter 2% Thoriated tungsten electrode for EN19 sheets.
The welding parameters used for this elding process both in pulsed current and non-pulsed current for two different thicknesses of the above material are given in Tables 4&5. The edge preparation and EN19 specimens are shown in figure 2.
After welding process is over, the radiography and liquid penetrant tests were conducted on the weldments(figure3),according to the ASTM standards , Section VIII, Division 2 for radiography and ASTM E-1417 for liquid penetrant test. The parameters used in the non-destructive testing are given in the Table 4.
Copyright to IJIRSET www.ijirset.com 1361
Fig.3 Fixture Fig.4 Root of the Welding
Fig.6 Lincoln Electrical square wave TIG 355 Fig.5 AC/DC Pulse Panel
Table 1. Chemical Compositions of work material EN19 alloy
Chemical Composition % wt
Material C Mn Si S P Ni Ti Cr Mo
Copyright to IJIRSET www.ijirset.com 1362
Table 2. Chemical Compositions of filler wire
Chemical Composition % wt
Material C Si Mn Mo Cr
ER80S-B2 0.08 0.5 0.5 0.5 1.3
Table 3. Mechanical properties EN19 at heat treated condition
Material UTS(MPa) 0.2% Y.S(MPa) % Elongation
EN19 Alloy >515 >480 >22
Table 4. Welding parameters for non-pulsed current welding of EN 19alloy
Weld Layer Filler Wire
Current I (amp) V (volts) ARC Travel
2 Root 1.6 DCSP 75 12 3.2
3 Root 1.6 DCSP 100 12 3.2
Ist pass 2.4 DCSP 100 12 3.5
Table 5. Welding parameters for pulsed current welding of EN19 Alloy steel
Material Thickness(mm) Weld Layer Filler Wire dia(mm) Pulse/Sec (Hz)
(amp) Ib (amp) V (volts) ARC Travel Speed(cm /min)
2 Root 1.6 2 DCSP 81 38 13 5.0
2 Root 1.6 4 DCSP 100 47 13 3.0
2 Root 1.6 6 DCSP 110 53 13 4.2
3 Root 1.6 2 DCSP 81 38 13 5.0
Ist pass 2.4 2 DCSP 124 58 13 4.1
3 Root 1.6 4 DCSP 100 47 13 3.0
Ist pass 2.4 4 DCSP 119 57 13 4.3
3 Root 1.6 6 DCSP 110 53 13 4.2
Copyright to IJIRSET www.ijirset.com 1363
Table 6. Radiography test parameters of EN 19 Alloy steel
EN19 Alloy steel
Voltage KV 65/100
Current (mA) 3.0
Time (min) 0.8
Film Used T-200
SFD (min) 0.7
Developer Time (min) 5.0
Stop Bath Time (min) 1.0
Fixer Time (min) 10
Table 7. Liquid Penetrant Test parameters of EN19 Alloy steel
EN19 Alloy steel
DP DIT MAGNA FLUX
Penetrant Used SKL-SP
Cleaner Used SKC-1
Developer Used SKD-S2
Dwell Time (at room temp) 10 min
Viewing Media Normal Light
Sensitivity 30 microns
Copyright to IJIRSET www.ijirset.com 1364
Fig.7 Welded joints of EN19 Alloy steel
Copyright to IJIRSET www.ijirset.com 1365
Fig.8 Radiographic images of EN19 Alloy steel weldments
III. RESULTS AND DISCUSSIONS
Table 8. The radiography test results of EN19 Alloy steel
S.No Material thickness Pulse/non-pulse welding Frequency(Hz) Observations
1 2.0 Non-pulse - No significance defect
2 2.0 Pulse 2 No significance defect
3 2.0 Pulse 4 One pores size 0.1mm
4 2.0 pulse 6 One pores size 0.4mm
5 3.0 Non-pulse -- One pores size 0.4mm
6 3.0 pulse 2 No significance defect
7 3.0 Pulse 4 Three pores size 0.1mm,0.1mm
8 3.0 pulse 6 Three pores size 0.2mm,0.2mm
Copyright to IJIRSET www.ijirset.com 1366 Table 9. The liquid penetrant test results of EN 19 alloy steel
S. No. Material thickness Pulse/non-pulse welding Frequency(Hz) observations
1 2.0 Non-pulse - No defect observed on welded area
2 2.0 Pulse 2 No defect observed on welded area
3 2.0 Pulse 4 No defect observed on welded area
4 2.0 pulse 6 No defect observed on welded area
5 3.0 Non-pulse -- No defect observed on welded area
6 3.0 pulse 2 No defect observed on welded area
7 3.0 Pulse 4 No defect observed on welded area
8 3.0 pulse 6 No defect observed on welded area
The parameters used in the NDT are presented in the tables 6 and 7. The average current , arc voltage and travel speed were kept constant i.e. the heat input per unit length in a weld is fixed , while pulse frequency and thickness of the sheet during the pulsed GTAW were varied.
A. EFFECT OF THICKNESS
The effect of thickness and welding parameters are given in the table 8&9 . During the radiography test no porosity was observed in 2.0 mm thick weldments welded at welding speed of 3.2cm/min in 2HZ,4HZ frequency. One porous of size 0.1mm and one porous of size 0.4mm were observed in the weldments welded with 4HZ and 6HZ frequencies respectively. In the 3mm weldments (non-pulsed) found one porous of size 0.4 mm .In 3mm thick weldments no porous was observed in the weldments welded with 2HZ. Three porous of size 0.1mm,0.1mm,0.4mm observed in the weldments of 4HZ, three porous of size 0.2mm,0.2mm and 0.3mm observed in the weldments of 6HZ.
The results shows that more porous found in higher thickness weldments with pulsed welding than the non pulsed current weldments, because the molten metal remains in solidification phase for the longer duration in non-pulsed then the gases are escaped and minimized the porous in the weldments, even though the porous sizes are within the acceptable limits, the observed porous can be minimized by proper supply of purging and shielding gases.
B. EFFECT OF FREQUENCY
Effect of pulsed frequency on the porosity during radiography are presented in the table 8, the porosity is measured in this present study in three frequencies i.e. 2HZ, 4HZ, 6 HZ. No porosity observed in weldments made at non frequency and 2HZ, whereas one pore size of 0.1 mm found in 4HZ weldment of 2mm thickness and one pore size of 0.4 mm found in weldments made at 6HZ, in 2mm thick weldments.
One pore of size 0.4mm found in 3mm thick weldments done at non-pulsed current. No significant defect found at 2HZ weldments.Three pores of size 0.1mm,0.1mm and and 0.4mm found in the weldments of 4HZ. Three pores of size 0.2mm, 0.2mm and 0.3mm found in the weldments made with 6HZ.
These results shows that porous size increased with the increase of frequency. This may be due to more vibration in weld torch and improper cleaning and supply of gases. The alloy steel EN19 contains porosity within the acceptable limits. No cracks were observed in liquid Penetrant test.
Copyright to IJIRSET www.ijirset.com 1367
 Troyer,W.,Tomsic,M.,and Barhotst, R , “Welding characteristics of Aluminium alloy ” welding journal,56(1),1977,26-32.
 Becker,D,W. and Adams, C.M, ”The role of pulsed GTA welding variables in solidification and grain refinement” welding journal,58(5)1979,134s-152s
 Becker,D,W. and Adams, C.M, “"Investigation of Pulsed GTA Welding parameters" welding journal,57(5)1978,134s-138s.  Omar,A.A, and Lundin, C.D,”welding journal”,58(4),1970,97s-104s.
 Tseng,C.F.and Savage,w,f, “The effect of oscillation” welding journal,50(11)1971,777-786.  Sharir,Y., Peiieg,J. and grill, “Metallurgical Technology”,5,1978, 190-196.
 Tsai, C.L., and Hou, C,A, "Theoretical Analysis of Weld Pool Behavior in the Pulsed Current GTAW Process", Heat Transfer,110, 1988, 160-165.
 Kate, S and Tanabe, S, "High speed welding of 0.5mm thickness alloy sheets using pulsed TIG welding", welding International 7, 1988, 602-608.
 Tsen, K.H. and Chou, C.P, “Effect of pulsed gas tungsten arc welding on angular distortion in austenitic stainless steel weldments”, science and Technology of welding and joining 6,(3),2001,149-153.
 Reddy,G.M.,Gokhale,A,A.and Prasad Rao K, "Effect of filler metal composition on weldability of Al-Li alloy 1441",Material Science&Technology,14,1998,61-66.
 Giridharam , P.M. and Muragan,N, “Sensitivity Analysis of pulsed current GTA welding process parameters on weldbead geometry”, National conference in advances in joining Technology 2004.
 Ramulu, M and Rubbert,M.P, “Gas Tungsten Arc welding of al-li-cu alloy 2090”, Welding Reaserach Supplement, 109s-114s.  Panwar, R.S., “Welding Engineering and Technology” p623
 ASTM , section VIII, Division VIII, Division II standards
Mr.Raveendra Akunuru is born in India, Andhra Pradesh. He received B.Tech (Mechanical) degree from R.E.C (Now National Institute of Technology) ,Warangal , Andhra Pradesh, India and M.Tech (Production Engineering) degree from Visveswaraya Technological University Belgaum, Karnataka, India. He is pursuing his doctoral study in Joining Processes at JNTU , Hyderabad, India. He is working as Associate Professor in Malla Reddy Engineering College, Secunderabad. He has 5 years of Industrial experience along with 10 years of Teaching experience. His research interests in Pulsed Current TIG Welding. He is a life member of Indian Welding Society.